# Supplementary Information (SI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2025

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_UM4052
_database_code_depnum_ccdc_archive 'CCDC 2440606'
loop_
_audit_author_name
_audit_author_address
'Peter Y. Zavalij'
;University of Maryland at College Park
United States of America
;
_audit_update_record             
;
2025-04-02 deposited with the CCDC.	2025-06-17 downloaded from the CCDC.
;
_audit_creation_date             2023-10-18
_audit_creation_method           
;
Olex2 1.5
(compiled 2023.03.06 svn.rbb2c1857 for OlexSys, GUI svn.r6748)
;
_shelx_SHELXL_version_number     2019/1

_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Fe2.98 Ga0.92 Te2'
_chemical_formula_sum            'Fe2.98 Ga0.92 Te2'
_chemical_formula_weight         485.84
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      hexagonal
_space_group_IT_number           194
_space_group_name_H-M_alt        'P 63/m m c'
_space_group_name_Hall           '-P 6c 2c'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-y, -x, -z+1/2'
'-x+y, y, -z+1/2'
'x, x-y, -z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z-1/2'
'x-y, -y, z-1/2'
'-x, -x+y, z-1/2'

_cell_length_a                   4.0724(3)
_cell_length_b                   4.0724(3)
_cell_length_c                   16.0928(15)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     231.13(4)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    2331
_cell_measurement_temperature    250(2)
_cell_measurement_theta_max      37.0
_cell_measurement_theta_min      2.5
_shelx_estimated_absorpt_T_max   0.776
_shelx_estimated_absorpt_T_min   0.071
_exptl_absorpt_coefficient_mu    26.658
_exptl_absorpt_correction_T_max  0.808
_exptl_absorpt_correction_T_min  0.065
_exptl_absorpt_correction_type   integration
_exptl_absorpt_process_details   '(Krause et al, 2015)'
_exptl_crystal_colour            black
_exptl_crystal_colour_primary    black
_exptl_crystal_density_diffrn    6.981
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             420
_exptl_crystal_size_max          0.21
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.01
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0318
_diffrn_reflns_av_unetI/netI     0.0170
_diffrn_reflns_Laue_measured_fraction_full 0.982
_diffrn_reflns_Laue_measured_fraction_max 0.988
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       4
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            2096
_diffrn_reflns_point_group_measured_fraction_full 0.982
_diffrn_reflns_point_group_measured_fraction_max 0.988
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.958
_diffrn_reflns_theta_min         2.531
_diffrn_ambient_temperature      250(2)
_diffrn_detector                 'PhotonIII C14 area detector'
_diffrn_detector_area_resol_mean 8.333
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Bruker D8Venture w/ PhotonIII'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_measurement_specimen_support 'MiTeGen loop'
_diffrn_orient_matrix_type       standard
_diffrn_orient_matrix_UB_11      0.0283285
_diffrn_orient_matrix_UB_12      0.0258287
_diffrn_orient_matrix_UB_13      0.0617520
_diffrn_orient_matrix_UB_21      0.2128951
_diffrn_orient_matrix_UB_22      -0.0553188
_diffrn_orient_matrix_UB_23      -0.0027199
_diffrn_orient_matrix_UB_31      0.1851132
_diffrn_orient_matrix_UB_32      0.2769048
_diffrn_orient_matrix_UB_33      -0.0063356
_diffrn_radiation_monochromator  'Helios optics'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'micro-source tube'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                151
_reflns_number_total             162
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.

 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'Apex4, Saint (Bruker, 2021)'
_computing_data_collection       'Apex4 (Bruker, 2021)'
_computing_data_reduction        'Apex4, Saint'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015c)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015a)'
_refine_diff_density_max         1.985
_refine_diff_density_min         -1.040
_refine_diff_density_rms         0.244
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.200
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     14
_refine_ls_number_reflns         162
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0319
_refine_ls_R_factor_gt           0.0282
_refine_ls_restrained_S_all      1.200
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0284P)²+4.1114P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0681
_refine_ls_wR_factor_ref         0.0694
_refine_special_details          -
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(Fe2) = Uanis(Fe3)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe1 Fe 0.333333 0.666667 0.750000 0.0101(8) Uani 0.903(14) 12 d S T P . .
Fe2 Fe 0.000000 0.000000 0.32704(9) 0.0107(4) Uani 1 6 d S T P . .
Fe3 Fe 0.000000 0.000000 0.500000 0.0107(4) Uani 0.070(8) 12 d S T P . .
Ga1 Ga 0.333333 0.666667 0.250000 0.0187(8) Uani 0.925(12) 12 d S T P . .
Te1 Te 0.333333 0.666667 0.59074(5) 0.0122(3) Uani 1 6 d S T P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1 Fe2 2.6581(7) 13_566 ?
Fe1 Fe2 2.6581(7) 4_665 ?
Fe1 Fe2 2.6581(7) 13_556 ?
Fe1 Fe2 2.6581(7) 13_666 ?
Fe1 Fe2 2.6581(7) 4 ?
Fe1 Fe2 2.6581(7) 4_565 ?
Fe1 Ga1 2.35121(17) 13_566 ?
Fe1 Ga1 2.35118(18) 13_666 ?
Fe1 Ga1 2.35121(17) 13_676 ?
Fe1 Te1 2.5629(8) . ?
Fe1 Te1 2.5629(8) 16_557 ?
Fe2 Fe2 2.480(3) 16_556 ?
Fe2 Fe3 2.7834(15) . ?
Fe2 Ga1 2.6581(7) . ?
Fe2 Ga1 2.6581(7) 1_545 ?
Fe2 Ga1 2.6581(7) 1_445 ?
Fe2 Te1 2.6979(8) 13_566 ?
Fe2 Te1 2.6979(8) 13_556 ?
Fe2 Te1 2.6979(8) 13_666 ?
Fe3 Te1 2.7678(4) . ?
Fe3 Te1 2.7678(4) 1_545 ?
Fe3 Te1 2.7678(4) 13_556 ?
Fe3 Te1 2.7678(4) 13_566 ?
Fe3 Te1 2.7678(4) 13_666 ?
Fe3 Te1 2.7678(4) 1_445 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Fe2 Fe1 Fe2 55.61(6) 13_566 4_565 ?
Fe2 Fe1 Fe2 100.00(4) 4_665 4 ?
Fe2 Fe1 Fe2 55.61(6) 4_665 13_666 ?
Fe2 Fe1 Fe2 55.61(6) 13_556 4 ?
Fe2 Fe1 Fe2 127.501(16) 4_565 13_666 ?
Fe2 Fe1 Fe2 100.00(4) 13_556 13_666 ?
Fe2 Fe1 Fe2 127.501(15) 4 13_666 ?
Fe2 Fe1 Fe2 100.00(4) 13_566 13_556 ?
Fe2 Fe1 Fe2 100.00(4) 4_565 4_665 ?
Fe2 Fe1 Fe2 100.00(4) 13_566 13_666 ?
Fe2 Fe1 Fe2 127.501(15) 13_556 4_665 ?
Fe2 Fe1 Fe2 127.501(16) 4_565 13_556 ?
Fe2 Fe1 Fe2 127.501(16) 13_566 4 ?
Fe2 Fe1 Fe2 100.00(4) 4_565 4 ?
Fe2 Fe1 Fe2 127.501(16) 13_566 4_665 ?
Ga1 Fe1 Fe2 152.20(3) 13_676 13_556 ?
Ga1 Fe1 Fe2 63.751(8) 13_666 13_666 ?
Ga1 Fe1 Fe2 63.751(8) 13_666 13_556 ?
Ga1 Fe1 Fe2 63.751(8) 13_676 4_665 ?
Ga1 Fe1 Fe2 63.751(8) 13_676 13_666 ?
Ga1 Fe1 Fe2 63.750(8) 13_566 13_566 ?
Ga1 Fe1 Fe2 63.751(8) 13_566 13_556 ?
Ga1 Fe1 Fe2 63.750(8) 13_566 4_565 ?
Ga1 Fe1 Fe2 152.20(3) 13_676 4 ?
Ga1 Fe1 Fe2 152.20(3) 13_566 13_666 ?
Ga1 Fe1 Fe2 63.750(8) 13_676 13_566 ?
Ga1 Fe1 Fe2 63.750(8) 13_676 4_565 ?
Ga1 Fe1 Fe2 152.20(3) 13_566 4_665 ?
Ga1 Fe1 Fe2 63.751(8) 13_666 4_665 ?
Ga1 Fe1 Fe2 63.751(8) 13_566 4 ?
Ga1 Fe1 Fe2 63.751(8) 13_666 4 ?
Ga1 Fe1 Fe2 152.20(3) 13_666 4_565 ?
Ga1 Fe1 Fe2 152.20(3) 13_666 13_566 ?
Ga1 Fe1 Ga1 120.0 13_666 13_566 ?
Ga1 Fe1 Ga1 120.0 13_566 13_676 ?
Ga1 Fe1 Ga1 120.0 13_666 13_676 ?
Ga1 Fe1 Te1 90.0 13_676 16_557 ?
Ga1 Fe1 Te1 90.0 13_566 . ?
Ga1 Fe1 Te1 90.000(1) 13_666 16_557 ?
Ga1 Fe1 Te1 90.0 13_666 . ?
Ga1 Fe1 Te1 90.0 13_566 16_557 ?
Ga1 Fe1 Te1 90.0 13_676 . ?
Te1 Fe1 Fe2 62.20(3) . 13_666 ?
Te1 Fe1 Fe2 117.80(3) . 4_665 ?
Te1 Fe1 Fe2 62.20(3) 16_557 4_565 ?
Te1 Fe1 Fe2 117.80(3) 16_557 13_566 ?
Te1 Fe1 Fe2 62.20(3) . 13_556 ?
Te1 Fe1 Fe2 117.80(3) . 4 ?
Te1 Fe1 Fe2 62.20(3) 16_557 4 ?
Te1 Fe1 Fe2 117.80(3) 16_557 13_556 ?
Te1 Fe1 Fe2 117.80(3) . 4_565 ?
Te1 Fe1 Fe2 62.20(3) . 13_566 ?
Te1 Fe1 Fe2 62.20(3) 16_557 4_665 ?
Te1 Fe1 Fe2 117.80(3) 16_557 13_666 ?
Te1 Fe1 Te1 180.0 16_557 . ?
Fe1 Fe2 Fe1 100.00(4) 13_556 13_566 ?
Fe1 Fe2 Fe1 100.00(4) 13_666 13_566 ?
Fe1 Fe2 Fe1 100.00(4) 13_556 13_666 ?
Fe1 Fe2 Fe3 117.80(3) 13_666 . ?
Fe1 Fe2 Fe3 117.80(3) 13_556 . ?
Fe1 Fe2 Fe3 117.80(3) 13_566 . ?
Fe1 Fe2 Ga1 52.498(15) 13_556 1_445 ?
Fe1 Fe2 Ga1 52.499(15) 13_556 1_545 ?
Fe1 Fe2 Ga1 52.499(15) 13_666 1_545 ?
Fe1 Fe2 Ga1 124.39(6) 13_556 . ?
Fe1 Fe2 Ga1 52.498(15) 13_666 . ?
Fe1 Fe2 Te1 127.892(4) 13_666 13_566 ?
Fe1 Fe2 Te1 127.892(5) 13_566 13_556 ?
Fe1 Fe2 Te1 127.893(4) 13_556 13_666 ?
Fe1 Fe2 Te1 127.892(4) 13_566 13_666 ?
Fe1 Fe2 Te1 127.893(4) 13_666 13_556 ?
Fe1 Fe2 Te1 127.892(4) 13_556 13_566 ?
Fe1 Fe2 Te1 57.170(16) 13_566 13_566 ?
Fe1 Fe2 Te1 57.171(16) 13_666 13_666 ?
Fe1 Fe2 Te1 57.171(16) 13_556 13_556 ?
Fe2 Fe2 Fe1 62.20(3) 16_556 13_666 ?
Fe2 Fe2 Fe1 62.20(3) 16_556 13_556 ?
Fe2 Fe2 Fe1 62.20(3) 16_556 13_566 ?
Fe2 Fe2 Fe3 180.0 16_556 . ?
Fe2 Fe2 Ga1 62.20(3) 16_556 . ?
Fe2 Fe2 Ga1 62.20(3) 16_556 1_545 ?
Fe2 Fe2 Ga1 62.20(3) 16_556 1_445 ?
Fe2 Fe2 Te1 119.37(3) 16_556 13_556 ?
Fe2 Fe2 Te1 119.37(3) 16_556 13_666 ?
Fe2 Fe2 Te1 119.37(3) 16_556 13_566 ?
Ga1 Fe2 Fe1 52.499(15) . 13_566 ?
Ga1 Fe2 Fe1 124.39(6) 1_445 13_666 ?
Ga1 Fe2 Fe1 52.499(15) 1_445 13_566 ?
Ga1 Fe2 Fe1 124.39(6) 1_545 13_566 ?
Ga1 Fe2 Fe3 117.80(3) 1_545 . ?
Ga1 Fe2 Fe3 117.80(3) 1_445 . ?
Ga1 Fe2 Fe3 117.80(3) . . ?
Ga1 Fe2 Ga1 100.00(4) . 1_545 ?
Ga1 Fe2 Ga1 100.00(4) 1_445 . ?
Ga1 Fe2 Ga1 100.00(4) 1_445 1_545 ?
Ga1 Fe2 Te1 178.44(6) 1_445 13_666 ?
Ga1 Fe2 Te1 178.44(6) 1_545 13_566 ?
Ga1 Fe2 Te1 80.985(10) 1_445 13_566 ?
Ga1 Fe2 Te1 80.984(10) 1_445 13_556 ?
Ga1 Fe2 Te1 80.985(10) 1_545 13_556 ?
Ga1 Fe2 Te1 80.984(10) . 13_666 ?
Ga1 Fe2 Te1 178.44(6) . 13_556 ?
Ga1 Fe2 Te1 80.985(10) 1_545 13_666 ?
Ga1 Fe2 Te1 80.984(10) . 13_566 ?
Te1 Fe2 Fe3 60.63(3) 13_666 . ?
Te1 Fe2 Fe3 60.63(3) 13_566 . ?
Te1 Fe2 Fe3 60.63(3) 13_556 . ?
Te1 Fe2 Te1 98.01(4) 13_666 13_556 ?
Te1 Fe2 Te1 98.00(4) 13_556 13_566 ?
Te1 Fe2 Te1 98.00(4) 13_666 13_566 ?
Fe2 Fe3 Fe2 180.0 13_556 . ?
Te1 Fe3 Fe2 58.156(14) 13_566 . ?
Te1 Fe3 Fe2 58.156(14) 1_445 13_556 ?
Te1 Fe3 Fe2 121.844(14) 13_566 13_556 ?
Te1 Fe3 Fe2 121.844(14) . . ?
Te1 Fe3 Fe2 58.156(14) 13_666 . ?
Te1 Fe3 Fe2 121.844(14) 13_666 13_556 ?
Te1 Fe3 Fe2 121.844(14) 1_545 . ?
Te1 Fe3 Fe2 58.156(14) 1_545 13_556 ?
Te1 Fe3 Fe2 121.844(14) 13_556 13_556 ?
Te1 Fe3 Fe2 121.844(14) 1_445 . ?
Te1 Fe3 Fe2 58.156(14) 13_556 . ?
Te1 Fe3 Fe2 58.156(14) . 13_556 ?
Te1 Fe3 Te1 94.728(19) 1_445 1_545 ?
Te1 Fe3 Te1 94.729(19) 13_556 13_666 ?
Te1 Fe3 Te1 85.271(19) 13_556 1_445 ?
Te1 Fe3 Te1 85.272(19) 13_666 1_545 ?
Te1 Fe3 Te1 94.729(19) . 1_445 ?
Te1 Fe3 Te1 94.729(19) . 1_545 ?
Te1 Fe3 Te1 94.728(19) 13_556 13_566 ?
Te1 Fe3 Te1 180.00(3) 13_566 1_545 ?
Te1 Fe3 Te1 85.272(19) 1_445 13_566 ?
Te1 Fe3 Te1 94.728(19) 13_666 13_566 ?
Te1 Fe3 Te1 85.272(19) 13_556 1_545 ?
Te1 Fe3 Te1 180.0 . 13_556 ?
Te1 Fe3 Te1 85.271(19) . 13_566 ?
Te1 Fe3 Te1 180.0 13_666 1_445 ?
Te1 Fe3 Te1 85.271(19) . 13_666 ?
Fe1 Ga1 Fe1 120.0 13_666 13_676 ?
Fe1 Ga1 Fe1 120.0 13_666 13_566 ?
Fe1 Ga1 Fe1 120.0 13_566 13_676 ?
Fe1 Ga1 Fe2 63.751(8) 13_666 1_665 ?
Fe1 Ga1 Fe2 63.750(8) 13_566 16_566 ?
Fe1 Ga1 Fe2 63.751(8) 13_676 16_666 ?
Fe1 Ga1 Fe2 63.751(8) 13_676 1_665 ?
Fe1 Ga1 Fe2 63.751(8) 13_566 . ?
Fe1 Ga1 Fe2 63.751(8) 13_666 . ?
Fe1 Ga1 Fe2 63.751(8) 13_566 16_556 ?
Fe1 Ga1 Fe2 63.750(8) 13_676 16_566 ?
Fe1 Ga1 Fe2 152.20(3) 13_566 1_665 ?
Fe1 Ga1 Fe2 63.750(8) 13_566 1_565 ?
Fe1 Ga1 Fe2 152.20(3) 13_676 . ?
Fe1 Ga1 Fe2 63.750(8) 13_676 1_565 ?
Fe1 Ga1 Fe2 152.20(3) 13_566 16_666 ?
Fe1 Ga1 Fe2 63.751(8) 13_666 16_556 ?
Fe1 Ga1 Fe2 152.20(3) 13_666 16_566 ?
Fe1 Ga1 Fe2 152.20(3) 13_666 1_565 ?
Fe1 Ga1 Fe2 63.751(8) 13_666 16_666 ?
Fe1 Ga1 Fe2 152.20(3) 13_676 16_556 ?
Fe2 Ga1 Fe2 55.61(6) 1_665 16_666 ?
Fe2 Ga1 Fe2 100.00(4) 1_565 1_665 ?
Fe2 Ga1 Fe2 55.61(6) . 16_556 ?
Fe2 Ga1 Fe2 55.61(6) 16_566 1_565 ?
Fe2 Ga1 Fe2 127.501(15) 16_556 1_665 ?
Fe2 Ga1 Fe2 100.00(4) 16_556 16_666 ?
Fe2 Ga1 Fe2 127.501(15) 16_566 1_665 ?
Fe2 Ga1 Fe2 100.00(4) . 1_565 ?
Fe2 Ga1 Fe2 127.501(15) 1_565 16_666 ?
Fe2 Ga1 Fe2 100.00(4) 16_566 16_666 ?
Fe2 Ga1 Fe2 127.501(15) . 16_566 ?
Fe2 Ga1 Fe2 100.00(4) . 1_665 ?
Fe2 Ga1 Fe2 127.501(15) 1_565 16_556 ?
Fe2 Ga1 Fe2 100.00(4) 16_566 16_556 ?
Fe2 Ga1 Fe2 127.501(15) . 16_666 ?
Fe1 Te1 Fe2 60.63(3) . 13_566 ?
Fe1 Te1 Fe2 60.63(3) . 13_666 ?
Fe1 Te1 Fe2 60.63(3) . 13_556 ?
Fe1 Te1 Fe3 121.844(14) . 1_565 ?
Fe1 Te1 Fe3 121.844(14) . 1_665 ?
Fe1 Te1 Fe3 121.844(14) . . ?
Fe2 Te1 Fe2 98.00(4) 13_566 13_666 ?
Fe2 Te1 Fe2 98.00(4) 13_566 13_556 ?
Fe2 Te1 Fe2 98.00(4) 13_666 13_556 ?
Fe2 Te1 Fe3 128.969(9) 13_666 . ?
Fe2 Te1 Fe3 61.21(3) 13_666 1_665 ?
Fe2 Te1 Fe3 128.969(9) 13_556 1_565 ?
Fe2 Te1 Fe3 128.969(9) 13_556 1_665 ?
Fe2 Te1 Fe3 128.969(9) 13_566 . ?
Fe2 Te1 Fe3 128.969(9) 13_666 1_565 ?
Fe2 Te1 Fe3 61.21(3) 13_556 . ?
Fe2 Te1 Fe3 61.21(3) 13_566 1_565 ?
Fe2 Te1 Fe3 128.969(9) 13_566 1_665 ?
Fe3 Te1 Fe3 94.730(19) 1_565 . ?
Fe3 Te1 Fe3 94.730(19) 1_565 1_665 ?
Fe3 Te1 Fe3 94.730(19) . 1_665 ?

_olex2_submission_special_instructions 'No special instructions were received'
